**Phase Transition Temperatures Through **

**Statistical Parameters By Image Analysis On **

**Py14BA:nFA Mesogens **

**Py14BA:nFA Mesogens**

Ch. Kamalakar1, C. J. Sreelatha1, D.M. Potukuchi2, S. Sreehari Sastry3*

Department of Physics, Kakatiya University, Warangal, Telangana, India**1**
Department of Physics, Acharya Nagarjuna University, Nagarjunanagar, India2
Department of Physics, Jawaharlal Nehru Technological University Kakinada, Kakinada, India3

**ABSTRACT**: Using statistical image analysis, phase transition temperatures of linear hydrogen-bonded liquid crystals
Py14BA:*n*FAs due to non liquid crystal (4-Pyridyl)*-*benzylidene-4’-*n-t*etradecyl aniline (Py14BA) and another non
liquid crystal aliphatic fatty acids (*n*FAs) where *n*= 12,14, and 16 are investigated. Textures of liquid crystals are
captured as a function of temperature using polarizing optical microscope attached with hot stage and camera. In this
image analysis, statistical parameters namely, mean, standard deviation, skewness and kurtosis of the liquid crystal
textures are computed using MATLAB software. The statistical parameters show abrupt changes and fluctuations as a
function of temperature which relates the phase transition of the sample. Statistical image analysis results are compared
with the literature values which are in good agreement.

**KEYWORDS**: Py14BA:*n*FA liquid crystals; Hydrogen bond; Transition Temperature; Image analysis; Statistical
Parameters** **

**I. INTRODUCTION **

The most spectacular and remarkable events in nature are the transformations between the various states of matter. Liquid crystal is a fourth state of matter, which is a transformation between the solid and conventional liquid. Phase transitions exhibited by these liquid crystal samples (Mesogens) are an important aspect of their properties and directly related to their structure in terms of molecular ordering [1]. These mesogens exhibits a multitude of transitions having new phases and studies of these phases have wide range applications on scientific fields. Each of the liquid crystal phases can form its own characteristic textures as a function of temperature which can be viewed under an polarizing optical microscope (POM). Identification of transition temperatures of these phases are important quantities that characterize the liquid crystal samples and is a necessary thing to study the physical properties of the material. The difference in transition temperatures between the melting and clearing point gives the range of stability of the liquid crystalline phase [2,3].

crystal samples which are viewed and recorded with the help of POM are used to identify the phase transition temperatures using image analysis technique.

**II. EXPERIMENTAL **

Non liquid crystal (4-Pyridyl)*-*benzylidene-4’-*n-t*etradecyl aniline (Py14BA) and non liquid crystal aliphatic fatty acids
(*n*FAs) formed liquid crystals through hydrogen bond liquid crystals of Py14BA:*n*FAs where *n*= 12,14, and 16 are
synthesized [5] and used. The experiment involved polarizing optical microscope (Meopta company) in the
arthroscopic mode attached with hot stage and high resolution colour camera for viewing and recording the textures as
a function of temperature [6]. The colour images or textures of given mesogens are recorded using camera with
resolution 2816x1880 pixels, which represents the 24bit true color pixel tone. Intensity values of the images are ranges
from 0 to 255 in Red, Green and Blue colours. The translated gray scale image is used for analysis and the defined
statistical parameters are computed using Matlab software.

**III. THEORY **

Statistical image analysis involves the computation of statistical parameters which extracts the information about the textural features of the image based on the gray level intensities of the image pixels. An image or texture

*I(i ,j)* is of size *m*-by-*n * is a two dimensional function and it is composed of *m* pixels in the vertical direction and

*n* pixels in the horizontal direction, *i, j *are horizontal and vertical co- ordinates of the image. The total number of
pixels in the image is *m*n = N, *

### 0

###

*i*

*m*

### , 0

###

*j*

###

*n*

. The defined statistical parameters are [7,8]
**(i)** **Mean: **

The mean (μ) is defined as the average level of intensity values of the image
or texture *I (i, j).*

*µ* =

###

*m*

*i*

*n*

*j*

*j*

*i*

*I*

*N*

1 1
### )

### ,

### (

### 1

(1)

** (ii) Standard Deviation: **

Standard Deviation of the image is defined as the square root of the variance. Variance measures the variability about the mean value of a image. If the value closer to mean, standard deviation is less.

Standard Deviation of an image:

### 1

### )

### )

### ,

### (

### (

1 1 2###

###

###

*N*

*j*

*i*

*I*

*m*

*i*

*n*

*j*

**

(2)
**(iii) Skewness**: It defines the symmetry around the mean intensity value.

3

1 1

3

### ( , )

### -(

### -1) *

*m* *n*

*i* *j*

*I i j*

*Skewness*

*N*

*S*

**

###

###

###

###

###

###

###

###

(3)**(iv) Kurtosis**: Kurtosis is a measure of peaked ness i.e. whether the intensity values are peaked or flat around the mean
intensity value.

4

1 1

4

### ( , )

### -(

### -1) *

*m* *n*

*i* *j*

*I i j*

*Kurtosis*

*N*

*S*

**

###

###

###

###

###

###

###

###

(4)

All the defined parameters are extremely sensitive to changes in the textural features of liquid crystals as a function temperature. Matlab software is used to compute the defined statistical parameters of the image. Image analysis using Matlab supports images generated by a wide range of devices, including digital camaras. The standard data and image formats include JPEG, JPEG-2000, TIFF, PNG etc. Matlab provides tools for image analysis tasks such as statistical analysis, features extraction and property measurement.

**IV. RESULTS AND DISCUSSION **

All the defined parameters are extremely sensitive to changes in the textural features of liquid crystals as a function temperature. Matlab software is used to compute the defined statistical parameters of the image. Image analysis using Matlab supports images generated by a wide range of devices, including digital camaras. The standard data and image formats include JPEG, JPEG-2000, TIFF, PNG etc. Matlab provides tools for image analysis tasks such as statistical analysis, features extraction and property measurement.

The present image analysis deals with the transition temperatures of hydrogen bonded liquid crystals Py14BA:*n*FAs where *n*= 12,14,
and 16. Textures of these compounds are recorded using polarizing optical microscope in arthroscopic mode attached to the high
resolution camera. The textures of liquid crystals are captured as a function of temperature, from the isotropic liquid state of the
sample to the crystalline state. On cooling the isotropic liquid of hydrogen bonded liquid crystals (HBLC) complexes, Py14BA:*n*FAs
exhibits monotropic nature in the case of (*n*=12,14) and found to bear glossy focal conic fan textures shown in Fig 1 which is
noticed as Smectic B crystal phase while *n*=16 exhibits enantiotropic nature with glossy focal conic fan texture Smectic B crystal
phase and marble threaded texture of Smectic F phase shown in Fig 2. The SmF phase exhibited by Py14BA:16FA remains till
ambient (∼30◦C) temperatures in the cooling cycle. The data of transition temperatures and the LC phases identified by the present
POM textural changes in heating and cooling cycles are presented in Table 1 .

** (a) (b) **

(a) (b)

Fig. 2. Optical textures of (4-Pyridyl)-benzylidene-4’-n-Tetradecyl aniline (Py14BA): long-chain aliphatic carboxylic
acid (FAs) nFAs (where n = 16)) liquid crystal. (a) Smectic B phase, (b) Smectic F phase of Py14BA:nFA where n=16
From, equations (1) to (4), statistical parameters of the liquid crystal textures are computed using MATLAB software.
Once the parameters are computed, the plots are drawn for parameters as a function of temperatures of the samples
from the isotropic state to the solid state and the plots are shown in Fig 3. On cooling, hydrogen bonded liquid crystals
Py14BA:*n*FAs undergoes a phase transition from the crystalline state to the isotropic state via an intermediate smectic
phase at different temperatures.

Table 1: Phases and Phase transition temperatures of Py14BA:*n*FA (where *n *=12,14, and 16)
Compound Phases Phase transition temperatures (oC)

POM and Image analysis DSC [5]

* *

* n *= 12 I – Sm B - K 61.9 - 52.0 - 49.0 62.6 - 49.96 – 43.0

* n* = 14 I – Sm B - K 68.0 - 63.5 -54.0 67.4- 64.60 - 55.0

* n *= 16 I – Sm B – Sm F - K 71.5-61.8-59.5 70.1-62.0-59.0

**( K:Crystal; sm B – Smectic B; sm F – Smectic F; I:Isotropic). **

**(a)** ** (b) **

** (c ) ** ** (d) **

Fig . 3. Statistical parameters of Py14BA:*n*FA (where *n *=12,14, and 16) (a) Mean; b) standard deviation;
(c) Skewness; (d) Kurtosis, as a function of temperature where the phase transitions are indicated.

*( K:Crystal; sm B – Smectic B; sm F – Smectic F; I:Isotropic). *

in graphical representation. Skewness arise due to the impact of sample size. . From Fig3(c), it is observed that tails of
the distribution and height of the graphical line for Py14BA:*n*FA samples are in the order of *n*=12>14>16 with
variation of temperature. It may be due to the impact of sample size, long aliphatic chain distribution and amphiphilic
interactions in the system. kurtosis constitutes a dimensionless measure of tail strength of a distribution, it depends on
the structure size, which actually depends on mean particle size in the sample. Kurtosis characterizes the uniformity of
height variations in graphical representation. From Fig 3(d), it is observed that tails of the distribution and height of the
graphical line for Py14BA:*n*FA samples are in the order of *n*=12>14>16 with variation of temperature. It may be due to
the impact of sample size, long aliphatic chain distribution and amphiphilic interactions in the system. Skewness and
kurtosis are the two dimension less parameters which are inter-related to each other.The behaviors of statistical
parameter curves of hydrogen bonded liquid crystals are different for different compounds. In the observed sequence,
there are pronounced variations in the respective phase transition temperatures and the clearing point of samples
decreases with increasing chain length. The observed transition temperatures of are in agreement with those reported in
the literature [5].Similar observation is reported [11]. The transition temperatures of Py14BA:*n*FA proposed method
and other technique (DSC) are shown in the table 1 which are in good agreement

**V. CONCLUSION **

Statistical parameters defined from the analysis of the textures as function of temperature is successful in identifying the liquid crystal phase transitions between the isotropic liquid phase to smectic phase and solid phase. Image analysis in conjunction with POM is a reliable and sensitive technique to identify phase transition temperatures of hydrogen bond liquid crystals.

**ACKNOWLEDGEMENTS **

The authors are thankful to Dr. K. Mallika for help in this work. One of the author (SSS) would like to acknowledge the UGC, New Delhi for providing BSR Faculty Fellow research grant No.F.18-1/2011 (BSR), dated January 4, 2017

**REFERENCES **

[1]. Shri Singh, “Phase transitions in liquid crystals”, 2000, Physics Report , 324, pp: 107 – 269.

[2] C.N. Rao and K.J. Rao, “Phase Transition in Solids : An Approach to the Study of the Chemistry and Physics of Solids”, McGraw-Hill, New York, 1978.

[3] D. Demus and L. Richter, “Textures of Liquid Crystals”, Verlag Chemie, New York, 1978.

[4] S. Sreehari Sastry, K.Mallika, B.Gowri Sankara Rao, Sie Tiong Ha and S.Lakshminarayana, “Identification of phase transition temperatures by statistical image analysis”, Liquid crystals,Volume: 39, pp: 695- 700, 2012.

[5] M. Muniprasad , M. Srinivasulu , P. V. Chalapathi & D. M. Potukuchi, *Mol. Cryst. Liq. Crys*, Volume.557, pp: 102–117, 2012.
[6] R. C. Gonzalez ;,P. Wintz, “Digital image processing,” Reading, MA: Addison- Wwesley,1987.

[7] Mahshid Roumi., (2009). “M.Sc. Thesis: Implementing Texture Feature Extraction Algorithms on FPGA”, Computer Engineering, Mekelweg 4, 2628 CD, Delft University of Technology, The Netherlands.

[8] B. Montrucchio, A. Sparavigna, and A. Strigazzi, “A new image method for enhancing the detection sensitivity of smooth transitions in crystals”, Liq. cryst, Volume. 24, pp. 841–852, 1998.

[9] J. Eccher, A.R. Sampaio, R.C. Viscovin, G. Conte, E. Westphal, H. Gallardo, and I.H. Bechtold, “Image processing as a tool for phase transitions identification”, Jounal of Molecular liquids, Volume. 153, pp.162–166, 2010.

[10] S. Sreehari Sastry, B. Gowri Sankara Rao, K. B. Mahalakshmi, K. Mallika , “Image Analysis Studies for Phase Transitions of Ferroelectric Liquid Crystals”,ISRN Materials Science, Vol.2012, pp:1-8, 2012.